Original article http://dx.doi.org/10.1590/1678-7757-2016-0233
0LV¿WDQGIUDFWXUHORDGRILPSODQW supported monolithic crowns in zirconia-reinforced lithium silicate
Abstract Rafael Soares GOMES1
Zirconia-reinforced lithium silicate (ZLS) is a ceramic that promises
to have better mechanical properties than other materials with the same
Carvalho de SOUZA2 Edmara Tatiely Pedroso BERGAMO1
indications as well as improved adaptation and fracture strength. Objective: ,QWKLVVWXG\PDUJLQDODQGLQWHUQDOPLV¿WDQGIUDFWXUHORDGZLWKDQGZLWKRXW thermal-mechanical aging (TMA) of monolithic ZLS and lithium disilicate (LDS)
crowns were evaluated. Material and methods: Crowns were milled using
Altair Antoninha DEL BEL CURY1
a computer-aided design/computer-aided manufacturing system. Marginal gaps (MGs), absolute marginal discrepancy (AMD), axial gaps, and occlusal gaps were measured by X-ray microtomography (n=8). For fracture load testing, crowns were cemented in a universal abutment, and divided into four groups: ZLS without TMA, ZLS with TMA, LDS without TMA, and LDS with TMA (n=10). TMA groups were subjected to 10,000 thermal cycles (5& DQGPHFKDQLFDOF\FOHV1+] $OOJURXSVZHUH subjected to compressive strength testing in a universal testing machine at a crosshead speed of 1 mm/min until failure. Student’s t-test was used to H[DPLQHPLV¿WWZRZD\DQDO\VLVRIYDULDQFHZDVXVHGWRDQDO\]HIUDFWXUH ORDGDQG3HDUVRQ¶VFRUUHODWLRQFRHI¿FLHQWVIRUPLV¿WDQGIUDFWXUHORDGZHUH calculated (D=0.05). The materials were analyzed according to Weibull GLVWULEXWLRQZLWKFRQ¿GHQFHLQWHUYDOV5HVXOWV$YHUDJH0*S and AMD (p=0.003) values were greater in ZLS than in LDS crowns. TMA did not affect the fracture load of either material. However, fracture loads of ZLS FURZQVZHUHORZHUWKDQWKRVHRI/'6FURZQVS )UDFWXUHORDGZDV moderately correlated with MG (r=-0.553) and AMD (r=-0.497). ZLS with TMA was least reliable, according to Weibull probability. Conclusion: Within the limitations of this study, ZLS crowns had lower fracture load values and JUHDWHUPDUJLQDOPLV¿WWKDQGLG/'6FURZQVDOWKRXJKWKHVHYDOXHVZHUH within acceptable limits.
Submitted: May 14, 2016 0RGL¿FDWLRQ6HSWHPEHU Accepted: October 28, 2016 Corresponding address: Altair Antoninha Del Bel Cury Department of Prosthodontics and Periodontology, Piracicaba Dental School, University of Campinas, Avenida Limeira 901, 13414-903 Piracicaba - São Paulo - Brazil 3KRQH)D[ e-mail: [email protected]
Keywords: Dental materials. Dental prosthesis. X-Ray microtomography.
1 Universidade Estadual de Campinas, Faculdade de Odontologia de Piracicaba, Departamento de Prótese e Periodontia, Piracicaba, SP, Brasil. 2 Universidade Estadual de Campinas, Faculdade de Odontologia de Piracicaba, Departamento de Odontologia Restauradora, Piracicaba, SP, Brasil.
J Appl Oral Sci.
strength20,21,28. The clinical success of a restoration can depend
The evolution of ceramic systems has been guided by efforts to enhance their strength and aesthetics32. The use of zirconia seemed to solve the problem of resistance in these systems, but the aesthetic quality of this material is less than desirable2. In the effort to obtain an aesthetic and strong material, a ceramic with 10% zirconia added to lithium silicate was recently developed and released19. Named zirconia-reinforced lithium silicate (ZLS), this material was designed for exclusive use with computer-aided design/computer-
on many factors, including fracture load, which can EHDIIHFWHGE\PDUJLQDOLQWHUQDO¿WDQGWKHDELOLW\WR withstand cyclic loading1,31,33. These properties need to be investigated in ZLS; studies testing the advantages attributed to this material remain scarce. This study ZDVFRQGXFWHGWRHYDOXDWHPDUJLQDODQGLQWHUQDOPLV¿W fracture load with and without thermal-mechanical aging (TMA), and reliability of ZLS compared with LDS. 7KHK\SRWKHVLVZDVWKDWWKH¿WDQGIUDFWXUHORDGRI ZLS would be superior to those of LDS.
aided manufacturing (CAD/CAM) systems. Its manufacturer claims that it is an outstanding aesthetic material, with more strength and easy milling ability
Material and methods
compared with lithium disilicate (LDS), generating optimized edge stability. Nevertheless, few studies supporting these features have been published6,19,30.
Specimens fabrication Using a three-dimensional (3D) optical scanning
LDS monolithic crowns have been used with
device (Ceramill Map400, Amann Girrbach, Koblach,
success . Monolithic crowns withstand greater
Vorarlberg, Austria), a 3D digital model of a morse
resistance than bi-layered crowns, and can be used
taper universal abutment (Munhão Universal, Intraoss,
in regions with greater masticatory forces . With
Itaquaquecetuba, São Paulo, Brazil) with a 4.5 mm
the application of extrinsic staining techniques, LDS
diameter, 6 mm height, and 2.5 mm collar height was
has been established as an aesthetic and strong
obtained. From this model, and regarding the anatomy
material . The use of ZLS in combination with CAD/
CAM technology appears to be another option for
drawn using CAD software (Ceramill Mind, Amann
restorative treatments with similar indications and
Girrbach). From this CAD model, 20 ZLS crowns
requirements as for LDS .
(Suprinity, Vita Zahnfabrik, Bad Säckingen, Baden-
CAD/CAM technology has facilitated restorative
Württemberg, Germany) and 20 LDS crowns (IPS
prosthetic treatment for clinicians and patients,
e.max CAD, Ivoclar Vivadent, Schaan, Liechtenstein)
decreasing restoration placement and overall chair
were milled (Ceramill Motion 2, Amann Girrbach).
times . Although the use of this technique has widely
Integrity of crown margins was examined by scanning
VSUHDG PLV¿W YDOXHV FDQ GLIIHU DPRQJ UHVWRUDWLRQV
electron microscopy (SEM) (JSM-5600LV, Jeol, Boston,
made with the same system and impression technique
due to material composition1,12,14,16. Material hardness FDQLQWHUIHUHZLWK¿WUHVXOWVDVKDUGHUPDWHULDOVFDQ PDNH WKH PLOOLQJ SURFHVV GLI¿FXOW OHDYLQJ FURZQV
susceptible to small fractures in very thin regions, such
material was evaluated using X-ray microtomography
as cervical areas14,17,25,27; thick and irregular cement
. In addition, some
USA). Each crown–universal abutment set was twice
studies have shown that the worse the adaptation of
wrapped for an adhesive tape that ran through on
the crown, the lower its resistance28,33.
the occlusal surface to the abutment’s base, avoiding
OLQHV FDQ DOVR FRPSURPLVH ¿W
any displacement, and positioned perpendicular to
remain a matter of debate. The most commonly
the X-ray source. The parameters used for image
acquisition were 80 kV, 1400 ms exposure time,
authors have claimed that thick cement layers may
lead to increased cement dissolution, microleakage,
each scan and reconstructed using NRecon software
localized stress accumulation, and reduction of fracture
(Bruker). Using DataView software (Bruker), central
DQG ǋP KDYH DOVR EHHQ UHSRUWHG
J Appl Oral Sci.
GOMES RS, SOUZA CMC, BERGAMO ETP, BORDIN D, DEL BEL CURY AA
coronal and sagittal slices were isolated from the
reconstructed images. Using CTAn software (Bruker),
Prior to cementation, the crowns (n=20 of each
the averages of the values obtained on each axis
material) were rinsed in 98% alcohol for 1 minute
were calculated. Following Holmes, et al.8 (1989),
in an ultrasonic bath. Their external surfaces were
four locations (centers of the buccal, lingual, mesial,
then protected with wax (New Wax, Technew, Rio
and distal faces) were selected for the evaluation
de Janeiro, Rio de Janeiro, Brazil), and the intaglio
of marginal gaps (MGs) and absolute marginal
surfaces were conditioned with 5% hydrofluoric
discrepancy (AMD; Figure 1A). Ten locations on
acid (Condac porcelana, FGM, Joinville, SC, Brazil)
each of the two slice types [four on the axial walls
for 20 seconds. The excess gel was removed with a
for the evaluation of axial gaps (AGs) and six on the
water jet, and the crowns were washed again in the
occlusal walls for the evaluation of occlusal gaps (OGs)
ultrasonic bath with 98% alcohol for 3 minutes. A thin
(Figure 1B)] were used for the evaluation of internal
layer of silane coupling agent (Prosil, FGM) was then
applied to the intaglio surfaces and allowed to act for 60 seconds; excess silane was volatilized with an air jet. The crowns were cemented into abutments that
Figure 1- A: Points used for the measurement of marginal gap (MG) and absolute marginal discrepancy (AMD). B: Points used for the measurement of axial gap (AG) and occlusal gap (OG) J Appl Oral Sci.
had been tightened into implant analogs28 (Titaoss Max
thermal cycles (MSCT-3e, Elquip, São Carlos, SP,
CM Analog, Intraoss) with 32 N.cm torque (TQ8800,
Brazil) in alternating water baths with temperatures
Lutron, Taipei, Taiwan) using a dual-cure resin
composite cement (Panavia F, Kuraray Noritake Dental
interval), amounting to about 65 seconds per cycle.
Inc., Okayama, Tokyo, Japan), and photopolymerized
For fracture load testing, a mechanical load
for 20 seconds/face using an LED source with 1000
was applied (Instron 4411, Instron, Norwood,
mW/cm² light intensity (VALO, Ultradent Products Inc,
M a s s a c h u s e t t s , U SA ) w i t h a s t a i n l e s s - s t e e l
South Jordan, Utah, USA).
hemispherical indenter (5 mm diameter) to the
The analogs were embedded in polyurethane resin
occlusal surface of each crown at a crosshead speed of
(F160, Axson Technologies, Saint Ouen I’Aumône,
or catastrophic fracture of the crown. After fracture,
in a metal matrix (20 mm diameter, 20 mm height).
all samples were submitted to fractographic analysis
Twenty crowns were used as the experimental groups
by SEM to identify the origin of failure4,22,23.
and the other 20 crowns served as controls. Ten crowns of each material were subjected to 1 million mechanical cycles (200 N load, 3.8 Hz frequency; ER-1300, ERIOS, São Paulo, SP, Brazil), with 10,000
Statistical analysis 0LV¿WDQGIUDFWXUHORDGGDWDZHUHDQDO\]HGXVLQJ the IBM SPSS Statistics 20 software (IBM Corp.,
Figure 2- A: Cervical area of the lithium disilicate crown with no chipping. B: Cervical area of the zirconia-reinforced lithium silicate crown, showing chipping at the edge (arrows) J Appl Oral Sci.
GOMES RS, SOUZA CMC, BERGAMO ETP, BORDIN D, DEL BEL CURY AA
$UPRQN1HZ0.05) or AG (r=-0.237, p>0.05), but it showed moderate negative correlations with MG (r=-0.553, p=0.026) and AMD (r=-0.49, p=0.05).
Discussion Studies on internal and marginal misfit of
Crowns presented catastrophic failure, exposing
monolithic ZLS crowns are scarce. The use of a non-
the abutment. Hackle lines, commonly formed when
Figure 4- Fractographic image showing fracture origin (O), direction of crack propagation (dcp), arrest lines (A), and hackle lines (H)
Figure 5- Weibull distribution showing failure probability according to the applied load J Appl Oral Sci.
GOMES RS, SOUZA CMC, BERGAMO ETP, BORDIN D, DEL BEL CURY AA
the great advantage of enabling evaluation of not only
μm according to most studies1,3,11-16,21,28. In addition,
the marginal area, but also the intaglio surface, while
the greatest discrepancy did not seem to compromise
preserving samples for further analyses (e.g., fracture
the mechanical behavior of the material a lot, since
load) with no effect on the results. It may, however,
moderate negative correlations were observed
be considered a costly and slow technique
between fracture load and MG and AMD.
,Q WKLV VWXG\ =/6 FURZQV VKRZHG KLJKHU PLV¿W
,QWHUQDO PLV¿W LV OHVV FRPPRQO\ HYDOXDWHG WKDQ
in the cervical region than did LDS crowns, which
PDUJLQDO PLV¿W *DSV ! P LQ D[LDO ZDOOV PD\
presented misfit values compatible with those
reduce the fracture strength of a crown16,17,25,27. In
the present study, AG values for both materials were
cervical region could be that a small amount of internal
P DQG $* ZDV QRW FRUUHODWHG ZLWK IUDFWXUH
space obstructs the settling of the crown , but this was
load. Another area of internal analysis is the occlusal
not observed in this study, since the two materials
produced similar internal adaptation values. A second
cementation due to polymerization shrinkage16. In this
hypothesis is that this difference could be due to the
occurrence of very small fractures during milling of
the cervical region in ZLS crowns . The results of this
not differ between materials12.
study support this hypothesis, as SEM images showed
Fracture loads were lower for ZLS crowns than
more irregularity in the cervical regions of ZLS crowns
for LDS crowns, with and without TMA. The presence
compared with LDS crowns, which may have increased
of zirconia in the microstructure seems to increase
WKH DYHUDJH PDUJLQDO PLV¿W RI =/6 FURZQV ,Q WKLV
material hardness, making it more prone to chipping
study was considered that there are no differences
during milling19. Chipping can worsen the adaptation
among abutment sizes, which could interfere also in
of the material and indirectly compromise fracture
the measurements outcomes.
Margin inaccuracy may be related to the increased
and fracture loads was detected in this study. TMA
brittleness index and chipping factor of ZLS, resulting
in greater marginal misfit, probably due to the
VHYHUDO SUHYLRXV UHSRUWV WKDW DJLQJ LQÀXHQFHV WKH
resistance of dental ceramics, although the Weibull
chipping factor (%) is the ratio of the total amount
probability curves showed that ZLS is affected more
of chipping around the marginal circumference of the
than LDS5,31,33. However, comparison of the present
restoration multiplied by 10027. It is positively related
results with those of other studies should be done
to the brittleness index, which is a ratio of hardness
with caution, given the poor standardization of
and fracture toughness. A higher hardness value and
loads, frequency, number of cycles, and substrates.
lower fracture toughness value increase the brittleness
In addition, Weibull probability can be unreliable in
index of a material, indicating that it is more prone
VPDOOVDPSOHVPDLQO\WKRVHZLWKQ 18, although
to chipping27. According to the manufacturers of the
presence of zirconia in the microstructure
materials used in this study, ZLS has a higher hardness
Both materials tested in this study resisted loads
value than does LDS in crystallized mode (7000 vs.
larger than maximum relative values of bite force
5600 MPa), and a lower fracture toughness value (2.00
found in the literature (~880 N)29. However, the
). However, no study has examined
fracture load test does not mimic failures occurring
these properties in the pre-crystalized phase, in which
when crowns are in clinical use4,5,33. The fractographic
these restorations are milled.
analysis conducted in the present study showed crack
vs. 2.25 MPa m
The occlusal and axial walls of ZLS and LDS crowns
propagation from the load point to the cervical area in
VKRZHG QR GLIIHUHQFH LQ PLV¿W 7KHVH WKLFN UHJXODU
all samples, opposite the direction of propagation in
areas may be less vulnerable to microfracture, thus
supporting the hypothesis that thin regions are more
results of the present study represent the real clinical
susceptible to damage during the milling process.
behavior of these materials.
Although ZLS presented a greater difference in PDUJLQDO PLV¿W FRPSDUHG ZLWK /'6 WKLV GHJUHH RI
J Appl Oral Sci.
The results of this study suggest that ZLS does not RXWSHUIRUP/'6LQWHUPVRIIUDFWXUHORDG¿WTXDOLW\RU
reliability. However, the effectiveness of this material
15- Park JK, Lee WS, Kim HY, Kim WC, Kim JH. Accuracy evaluation of
metal copings fabricated by computer-aided milling and direct metal laser sintering systems. J Adv Prosthodont. 2015;7(2):122-8. 16- Pimenta MA, Frasca LC, Lopes R, Rivaldo E. Evaluation of PDUJLQDODQGLQWHUQDO¿WRIFHUDPLFDQGPHWDOOLFFURZQFRSLQJVXVLQJ x-ray microtomography (micro-CT) technology. J Prosthet Dent.
2015;114(2):223-8. 17- Quinn GD, Giuseppetti AA, Hoffman KH. Chipping fracture
Within the limitations of this study, ZLS crowns had lower fracture load values and greater marginal
resistance of dental CAD/CAM restorative materials: Part I, procedures and results. Dent Mater. 2014;30(5):e112-23. 18- Quinn JB, Quinn GB. A practical and systematic review of Weibull
statistics for reporting strengths of dental materials. Dent Mater.
all values were within the limits considered to be
acceptable. Thus, both materials comply with the indication criteria.
19- Ramos NC, Campos TM, La Paz IS, Machado JPB, Bottino MA, Cesar PF, et al. Microstructure characterization and SCG of newly engineered dental ceramics. Dent Mater. 2016;32(7):870-8 20- Rojpaibool T, Leevailoj C. Fracture resistance of lithium disilicate ceramics bonded to enamel or dentin using different resin cement types DQG¿OPWKLFNQHVVHV-3URVWKRGRQW
21- Rungruanganunt P, Kelly JR, Adams DJ. Two imaging techniques IRU'TXDQWL¿FDWLRQRISUHFHPHQWDWLRQVSDFHIRU&$'&$0FURZQV
1- Anadioti E, Aquilino SA, Gratton DG, Holloway JA, Denry IL, 7KRPDV*:HWDO,QWHUQDO¿WRISUHVVHGDQGFRPSXWHUDLGHGGHVLJQ computer-aided manufacturing ceramic crowns made from digital and conventional impressions. J Prosthet Dent. 2015;113(4):304-9. 2- Baldissara P, Llukacej A, Ciocca L, Valandro FL, Scotti R. Translucency of zirconia copings made with different CAD / CAM systems. J Prosthet Dent. 2010;104(1):6-12. 3- Borba M, Miranda WG Jr, Cesar PF, Griggs JA, Della Bona A. Evaluation RIWKHDGDSWDWLRQRI]LUFRQLDEDVHG¿[HGSDUWLDOGHQWXUHVXVLQJPLFUR CT technology. Braz Oral Res. 2013;27(5):396-402. 4- Campos RE, Soares P V, Versluis A, Júnior OB, Ambrosano GM, Nunes IF. Crown fracture: failure load, stress distribution, and fractographic analysis. J Prosthet Dent. 2015;114(13):447-55. 5- Coelho PG, Bonfante EA, Silva NRF, Thompson VP. Laboratory simulation of Y-TZP all-ceramic crown clinical failures. J Dent Res. 2009;88(4):382-6. 6- Elsaka SE, Elnaghy AM. Mechanical properties of zirconia reinforced lithium silicate glass-ceramic. Dent Mater. 2016;32(7):908-14. 7- Herrguth M, Wichmann M, Reich S. The aesthetics of allceramic veneered and monolithic CAD/CAM crowns. J Oral Rehabil. 2005;32(10):747-52. 8- Holmes JR, Bayne SC, Holland GA, Sulik WD. Considerations in PHDVXUHPHQWRIPDUJLQDO¿W-3URVWKHW'HQW +XQJ6++XQJ.6(LFN-'&KDSSHOO530DUJLQDO¿WRISRUFHODLQ fused-to-metal and two types of ceramic crown. J Prosthet Dent. 1990;63(1):26-31. 10- International Organization for Standardization. ISO 14801: dynamic fatigue test for endosseous dental implants. Geneva: The Organization; 2007. 11- Liu B, Lu C, Wu Y, Zhang X, Arola D, Zhang D. The effects of adhesive type and thickness on stress distribution in molars restored with all-ceramic crowns. J Prosthodont. 2011;20(1):35-44. 12- Mously HA, Finkelman M, Zandparsa R, Hirayama H. Marginal and internal adaptation of ceramic crown restorations fabricated with
J Dent. 2010;38(12):995–1000. 22- Scherrer SS, Quinn JB, Quinn GD, Kelly JR. Failure analysis of ceramic clinical cases using qualitative fractography. Int J Prosthodont. 2006;19(2):185-92. 23- Scherrer SS, Quinn JB, Quinn GD, Wiskott HW. Fractographic ceramic failure analysis using the replica technique. Dent Mater. 2007;23(11):1397-404. 24- Schultheis S, Strub JR, Gerds TA, Guess PC. Monolithic and biOD\HU &$'&$0 OLWKLXPGLVLOLFDWH YHUVXV PHWDOFHUDPLF ¿[HG GHQWDO prostheses: Comparison of fracture loads and failure modes after fatigue. Clin Oral Investig. 2013;17(5):1407-13. 25- Song X, Ren H, Yin L. Machinability of lithium disilicate glass ceramic in in vitro dental diamond bur adjusting process. J Mech Behav Biomed Mater. 2016;53:78–92. 26- Sulaiman TA, Delgado AJ, Donovan TE. Survival rate of lithium disilicate restorations at 4 years: a retrospective study. J Prosthet Dent. 2015;114(3):364-6. 27- Tsitrou EA, Northeast SE, van Noort R. Brittleness index of machinable dental materials and its relation to the marginal chipping factor. J Dent. 2007;35(12):897-902. 28- Tuntiprawon M, Wilson PR. The effect of cement thickness on the fracture strength of all-ceramic crowns. Aust Dent J. 1995;40(1):17-21. 29- Van der Bilt A. Assessment of mastication with implications for oral rehabilitation: a review. J Oral Rehabil. 2011;38(10):754-80. 30- Weyhrauch M, Igiel C, Scheller H, Weibrich G, Lehmann KM. Fracture strength of monolithic all-ceramic crowns on titanium implant abutments. Int J Oral Maxillofac Implants. 2016;(31)2:304-9 31- Yang R, Arola D, Han Z, Zhang X. A comparison of the fracture resistance of three machinable ceramics after thermal and mechanical fatigue. J Prosthet Dent. 2014;112(4):878-85. =KDQJ